Abstract
Point defects in hexagonal boron nitride (hBN) have attracted growing attention as bright singlephoton emitters. However, understanding of their atomic structure and radiative properties remains incomplete. Here we study the excited states and radiative lifetimes of over 20 native defects and carbon or oxygen impurities in hBN using ab initio density functional theory and GW plus BetheSalpeter equation calculations, generating a large data set of their emission energy, polarization and lifetime. We find a wide variability across quantum emitters, with exciton energies ranging from 0.3 to 4 eV and radiative lifetimes from ns to ms for different defect structures. Through a Bayesian statistical analysis, we identify various highlikelihood chargeneutral defect emitters, among which the native V_{N}N_{B} defect is predicted to possess emission energy and radiative lifetime in agreement with experiments. Our work advances the microscopic understanding of hBN singlephoton emitters and introduces a computational framework to characterize and identify quantum emitters in 2D materials.
Similar content being viewed by others
Introduction
Twodimensional (2D) materials are rapidly growing as a platform for photon based quantum information technologies^{1,2}. The discovery of singlephoton emitters (SPEs) at point defects in hBN^{3} has spurred an intense search for optically active defects in 2D crystals^{4}. Compared to defects in bulk crystals, such as diamond and silicon carbide^{5,6,7,8}, defects embedded in 2D materials promise to be more easily addressed and controlled. In the case of hBN, defect emitters exhibit a range of desirable properties, including high emission rate, room temperature stability, strong zerophonon line (ZPL) and easy integration with other optical components using 2D hBN crystals^{1,9,10,11,12}.
A pressing challenge for defect emitters in hBN is identifying their atomic structure. Various possible structures have been proposed on the basis of density functional theory (DFT) calculations and their comparison with experiments^{3,13,14,15,16,17,18,19}. However, while DFT can provide valuable insight into the formation energy, symmetry and electronic structure of SPE defects, it cannot address key aspects of pointdefect SPEs such as their excited states and radiative processes responsible for light emission. To complicate the matter further, similar to other 2D materials and their defects^{20,21,22}, optical transitions at defects in hBN are dominated by excitonic effects^{23}, which require specialized firstprinciples calculations beyond the scope of DFT. Quantum chemistry approaches and density matrix renormalization group have also been used to investigate specific defect structures^{24,25}, but wide comparisons among different structures are still missing.
The BetheSalpeter equation (BSE) can accurately predict optical properties and excitons in materials^{26}. It also enables, due to recent advances, precise calculations of radiative lifetimes in 2D and bulk crystals^{27,28,29,30}. The radiative lifetime plays an important role in the study of SPEs as it determines the shortest decay time constant in the secondorder photon correlation function^{31,32} and can also be measured directly from fluorescence intensity decay^{3,10}. Applying the BSE and related methods to defect emitters in hBN would enable direct comparisons between theory and experiment of the emission energy and radiative lifetime, providing valuable information to identify defect SPEs. Yet, firstprinciples BSE calculations are computationally costly to carry out on defect structures, and the radiative lifetime calculations are only a recent development.
In this work, we employ the BSE approach to compute from first principles the optical properties, transition dipoles, excitons and radiative lifetimes of atomic defects in hBN. We examine a large pool of candidate SPE structures, spanning native defects and carbon or oxygen impurities, to correlate their atomic structures with their photophysics. We find that different quantum emitters exhibit radiative lifetimes spanning six orders of magnitude and emission energies from infrared to ultraviolet. Bayesian statistical analysis is employed to correlate our results with experiments and identify highlikelihood chargeneutral SPEs in hBN, among which we find the V_{N}N_{B} defect to have the highest likelihood. Indepth calculations on the V_{N}N_{B} defect highlight the strong dependence of its radiative properties on small perturbations to its atomic structure. The dependence of the defect radiative properties on dielectric screening is analyzed by comparing monolayer and bulk hBN results. Our systematic investigation addresses key challenges for characterizing the excited states and radiative properties of defect emitters in 2D materials.
Results
Excited state properties of hBN defect emitters
Our candidate defect structures consist of chargeneutral native defects and carbon or oxygen impurities occupying one or two atomic sites, for a total of 8 different native defects and 7 structures for each of carbon and oxygen impurities. We compute the ground state defect properties using DFT, employing fully relaxed defect atomic structures in 5 × 5 supercells of monolayer hBN (and for some defects, in bulk hBN). We then refine the electronic structure of selected defects using GW calculations^{33}, followed by BSE calculations to obtain the exciton energies and wave functions and from them the optical absorption, transition dipoles and radiative lifetimes (see the “Methods” section). In the following, we denote the defects in hBN as X_{N}Y_{B} if neighboring N and B atoms are replaced by species X and Y, respectively, where X and Y can be a vacancy (denoted as V) or another element^{3,13}. We focus on emitters in the interior of the 2D crystal^{34,35} and do not consider defects that would likely appear at the sample edges or corners^{36,37}.
The electronic energies obtained using DFT, while in general not representative of electronic or optical transitions, can be used for estimating qualitative trends. Figure 1 shows the lowest (HOMOLUMO) spinconserving transition energy of the candidate defects, obtained from DFT, together with the emission polarization inferred from structural symmetry. The defect structures considered here exhibit three different types of local symmetries, D_{3h}, C_{2v}, and C_{s}. In the high symmetry D_{3h} structure, adopted by N_{B}, V_{N}, B_{N}, C_{B}, C_{N}, O_{N}, emitted light cannot be linearly polarized. Conversely, linearly polarized emitted light, as observed experimentally in hBN SPEs^{11}, is possible in the C_{2v} and C_{s} symmetries. In the C_{2v} configuration, which is the most common among the defects investigated here, the threefold rotational symmetry is broken but all the atoms remain inplane, preserving the mirror symmetry with respect to the crystal plane. The C_{s} symmetry found in the V_{N}N_{B}, V_{N}C_{B}, V_{N}O_{B} and O_{B} defects is instead associated with an outofplane distortion that breaks the mirror symmetry about the plane. The DFT transition energies for the 22 defect structures range from 0 to 3.5 eV. In contrast, the ZPL of the measured SPEs are in the 1.6−2.2 eV energy range^{11}, as shown by the shaded region in Fig. 1. While candidate structures with D_{3h} symmetry can be ruled out, C_{2v} and C_{s} structures with exceedingly small or large DFT transition energies also appear unlikely on the basis of the DFT results.
Starting from the DFT ground state, for selected defects we compute the excited state properties with the GWBSE method, obtaining the quasiparticle energies in the oneshot G_{0}W_{0} approximation and the exciton energies and wave functions with the BSE, which captures electronhole interaction and excitonic effects. We combine the solutions of the BSE with an approach we recently developed^{29,30} to compute the radiative lifetime of an exciton state from Fermi’s golden rule. Generalizing our previous formula for isolated (0D) emitters^{29} to include anisotropic dielectric screening in hBN, the radiative decay rate γ_{S} of an exciton state S is:
where ϵ_{xy}(k_{xy}) and ϵ_{z} are the inplane and outofplane dielectric function of hBN, respectively, k_{xy} is the inplane photon wavevector, E_{S} is the exciton energy and p_{S,xy} and p_{S,z} are the corresponding components of the exciton transition dipole. The radiative lifetime τ_{S} below is defined as the inverse of γ_{S} and accounts only for the radiative decay channel. We use a constant inplane dielectric function for bulk hBN (ϵ_{xy} = 5) at optical wavelengths, and for monolayer hBN we take into account the dependence on wavevector k as ϵ_{xy}(k) ≈ 1 + 2πα_{2D} ∣k∣^{38}, where α_{2D} is a constant equal to 0.4 nm^{39}. In this approach, which is appropriate for 2D materials, the inplane dielectric function of monolayer hBN reduces to a value of 1 at optical photon wavelengths.
Figure 2 shows the computed radiative lifetimes and lowest bright exciton energies for nine selected defects, including V_{N}, B_{N}, V_{N}N_{B}, C_{N}, V_{N}C_{B}, C_{N}V_{B}, O_{B}, O_{N}V_{B}, and V_{B}O_{N}. We find that the exciton energy can differ significantly−by as much as 1 eV− from the corresponding DFT transition energy, which fails to account for screening and electronhole interaction effects. This result is a testament to the importance of excited state calculations for investigating SPEs. Surprisingly, we find that the computed radiative lifetime for the selected structures span six orders of magnitude, from about 1 to 10^{6} ns (1 ms), showing that the emission rate and brightness of quantum emitters in hBN can vary widely. The values typically found in experiments for the emission energy (1.6−2.2 eV) and radiative lifetime (1−10 ns) are also given for comparison in Fig. 2.
Writing the exciton transition dipole in Eq. (1) as p_{S} = − (imE_{S}/ℏe) × e r_{S}, with \(\left{{\bf{r}}}_{S}\right=\left\left\langle 0\right{\bf{r}}\leftS\right\rangle \right\) to highlight its physical meaning of an atomicscale dipole, and setting \(\left{{\bf{r}}}_{S}\right\) equal the BN bond length, we obtain an upper bound estimate of the exciton transition dipole (of 6.9 Debye) because the excitons considered here are tightly bound to the defect. The resulting radiative lifetime as a function of exciton energy, as shown by the blue line in Fig. 2, gives an approximate lower bound to the calculated radiative lifetimes. Our calculated exciton energies and radiative lifetimes clearly follow the trend set by this lower bound. The physical insight of this analysis is that due to incomplete overlap of the electron and hole wavefunctions, the exciton transition dipole for most defects is significantly smaller than the bond length, leading to longer radiative lifetimes than this theoretical bound. We note that the experimental emission energies and lifetimes for defect emitters in hBN, indicated by the gray area in Fig. 2, fall almost entirely below this lower bound, suggesting that nonradiative decay processes need to play an important role if atomic point defects like the ones discussed here are responsible for SPE.
Bayesian analysis of the likelihood of candidate defect structures
As the candidate defect structures have properties distributed across a wide range, it is challenging to pinpoint the correct defect structure from our results. As such, we pursue a quantitative analysis of the relative likelihood of the various structures using Bayesian inference, a statistical approach for dealing with uncertainties and combining information from different categories, in which the likelihood of a hypothesis is updated as more evidence or information becomes available^{40}. The workflow of our analysis is shown in Fig. 3. We first generate candidate structures by systematically enumerating all possible structures where n adjacent atomic sites are replaced by a vacancy, antisite or impurity point defect. We then obtain the list of defects studied in our work by considering structures with n = 1 or 2 replacements, as defects spanning multiple sites are typically less likely to occur. We use carbon and oxygen as the impurity elements, the most likely impurities in hBN according to the current literature. This list of candidates includes structures similar to known solidstate quantum emitters such as the NV and SiV centers in diamond, and includes most of the hBN defect emitters proposed in the literature so far^{13,14,15,16,17,18,19} as well as additional structures that were not previously considered.
A prior likelihood p(h) is then assigned to each candidate structure h as an initial guess of how likely it is that the defect structure can appear in the hBN crystal. The prior likelihood can be tailored to describe various experimental scenarios. For example, if carbon impurities are added in the experiment, as shown in recent work^{41}, one could include the presence of a carbon impurity in the prior likelihood, therefore favoring the posterior likelihood of carboncontaining emitters. Here, without referring to specific experimental conditions, we choose the prior likelihood p(h) on the basis of the structural complexity of the defect, using the single exponential form \(p(h)\propto {S}_{h}{A}^{{C}_{h}}\), where C_{h} measures the complexity of the structure, defined as the number of vacancies and antisite defects plus twice the number of impurities, A is a constant, and S_{h} is a degeneracy factor due to symmetryrelated configurations.
We subsequently combine our computational results with experimental evidence to obtain a posterior likelihood p(h∣E) for each structure^{40}:
where the likelihood function p(E∣h) is the likelihood that the structure h is compatible with a specific piece of experimental evidence E on the basis of our calculations. The resulting posterior likelihood, which is updated in multiple steps using several computed properties, quantifies which structures among those considered are more likely to be defect emitters in hBN.
The properties of the candidate SPE defects and the results of our Bayesian inference analysis are summarized in Table 1. Moving in the table from left to right, the prior likelihood p(h) is updated to posterior likelihood p(h∣E) using calculations presented in subsequent columns. The first computed posterior likelihood, p_{1}(h∣E), uses the DFT results to infer whether the defect symmetry is compatible with linearly polarized emission and whether the DFT transition energy, within a standard deviation of ~0.5 eV, falls in the 1.6−2.2 eV emission range found in experiments^{10,11,34}. The final posterior likelihood p_{2}(h∣E) in the rightmost column of Table 1 gives the likelihood of the most likely defect structures when all factors have been taken into account, including comparison between the lowest bright exciton energy and the experimental emission energy, and comparison with experiment of the radiative lifetime from our GWBSE calculations. We emphasize that the absolute value of the likelihood is arbitrary and a value of 1 does not imply certainty. The likelihood shown in Table 1 is normalized so that the maximum value on each column is 1. The detailed rationale of our Bayesian analysis is described in the Supplementary Note 3.
The main finding from the data in Table 1 is that the V_{N}N_{B} defect, which was originally proposed as a SPE in hBN on the basis of DFT calculations^{3,13,18}, possesses optical and radiative properties that most accurately match the experimental results, even after taking into account excitonic effects and radiative lifetimes. The next most likely structure is the oxygen impurity defect, O_{B}, with an emission energy of 1.52 eV, just below the experimental range. On the other hand, we find that the V_{N}C_{B} defect, which is also considered a likely candidate in the literature based on DFT calculations^{13,18}, has an emission energy of 2.6 eV that lies too far above the experimental energy range when excitonic effects are included, making it a less likely candidate. Although our analysis excludes V_{N}C_{B} and other defects with higher emission energies as candidates for the 1.6−2.2 eV SPEs, these structures may still be good candidates for SPEs in the ultraviolet range^{42,43}. As the most likely defect emitter in hBN is the V_{N}N_{B} structure according to our analysis, we investigate it in more detail to better understand its radiative properties.
Figure 4(a) shows that the relaxed atomic structure of the V_{N}N_{B} defect in monolayer hBN exhibits an outofplane displacement of the central nitrogen (N) atom by z = 0.66 Å. If the structure is made planar by constraining the N atom to the hBN plane, the total energy of the system is only moderately higher (by 0.125 eV) than the equilibrium structure. Therefore the total energy forms a shallow doublewell potential as a function of the outofplane N atom displacement. Consistent with recent findings^{44}, this small energy difference suggests that the structure is soft in the outofplane direction and could fluctuate due to external perturbations.
To take this result into account, we compute the optical absorption spectrum of the V_{N}N_{B} defect for outofplane displacements z of the N atom in the 0−0.83 Å range, interpolating between the inplane and outofplane equilibrium structures to obtain the intermediate metastable structures. We find that the absorption spectrum changes drastically even for small changes of z, as shown in Fig. 4(c). The spectrum is dominated by two exciton absorption peaks at low energy. At the equilibrium position (z = 0.66 Å), the first peak at 1.92 eV is associated with a transition from the top valence to the bottom conduction spinmajority electronic states, whose wave functions are shown in Fig. 4(b). As the displacement z of the N atom is decreased from the equilibrium value to zero, which corresponds to a planar structure, the energy of the first exciton peak decreases at first but then increases again at small z values while gaining oscillator strength monotonically. The second peak at 2.7 eV is also due to a transition from the top valence to the bottom conduction spinminority bands with relatively large oscillator strength at the outofplane equilibrium N atom position. Both the energy and the oscillator strength of this peak decrease monotonically as z decreases [see Fig. 4(c)]. For the planar structure (z=0), the second peak becomes the lowestenergy transition but completely loses its oscillator strength and becomes a dark state.
These significant changes in the two lowestenergy exciton peaks are accompanied by substantial changes in the exciton radiative lifetimes. Although the lifetime of the lowest exciton is 334 ns for the DFT equilibrium outofplane distortion, it becomes only 19 ns if the V_{N}N_{B} structure is kept planar (z = 0 case), as shown in Fig. 4(d). This value of the radiative lifetime for the planar structure is within a factor of 2−3 of experimental results^{11}. Because many experiments are carried out on thicker hBN samples, we also calculated the radiative lifetime of the V_{N}N_{B} defect embedded in bulk hBN (instead of monolayer), a setting resembling more closely SPE experimental measurements in thicker hBN samples (see the “Methods” section). Due to interlayer interactions, the outofplane displacement of the N atom is reduced to 0.45 Å in bulk hBN. Going from monolayer to bulk reduces the radiative lifetime of the V_{N}N_{B} defect to 147 ns due to changes in the dielectric environment and transition dipole, both of which affect the radiative emission rate in Eq. (1). This result shows that different dielectric environments, for example due to the use of different substrates, may have a strong impact on the radiative properties of the defect. Therefore we conclude that the radiative lifetime of the V_{N}N_{B} defect is highly sensitive to both outofplane structural distortions and the dielectric environment.
Discussion
While our computed lifetimes are in the 20−350 ns range for different V_{N}N_{B} structures, these values pertain to an ideal defect with 100% quantum yield, whereas defect emission measured so far in hBN is likely associated with a lower quantum yield. To explain the discrepancy between the experimental and calculated lifetimes, note that nonradiative processes, which are not included in our calculation of intrinsic radiative lifetimes, could significantly reduce the apparent lifetime measured in experiments. For example, a defect with a measured 10 ns lifetime but only a 10% quantum yield would correspond to a 100 ns intrinsic radiative lifetime in the same range as our computed values. Future SPE measurements in hBN taking into account the quantum yield may provide a better estimate of the intrinsic SPE radiative lifetime and enable a more accurate comparison with our calculations.
In our study, we did not take into account the FrankCondon shift or excitonphonon coupling effects such as zeropoint renormalization, which are beyond the scope of this work. Although these effects may cause small shifts of the exciton energy and lead to broadening or satellite peaks^{45,46}, the overall transition dipole remains the same within the FrankCondon approximation, and thus we expect minimal changes in the radiative lifetimes due to these effects. Note also the possible presence of charged defects in experiments^{4}, which are not considered in this work.
In summary, we have investigated the excited state and radiative properties of many candidate defect SPEs in hBN. Our calculations address the photophysics of these defect structures, including their optical transitions and radiative lifetimes, using calculations that accurately account for excitonic effects and anisotropic dielectric screening. Our Bayesian statistical analysis allows us to identify the native V_{N}N_{B} defect as the most likely candidate within a wide pool of over 20 chargeneutral native defects and carbon or oxygen impurities. This work explores the fertile ground at the intersection of excitedstate firstprinciples calculations and Bayesian learning methods, and the application of this framework to quantum technologies. The search for solidstate quantum emitters will greatly benefit from such precise firstprinciples calculations of excited states in materials.
Methods
Details of the firstprinciples calculations
We carry out DFT calculations in the generalized gradient approximation using the PerdewBurkeErnzerhof (PBE) exchangecorrelation functional^{47}. Our spinpolarized DFT calculations employ the planewave pseudopotential method implemented in Quantum Espresso^{48}. The defects are placed in a 5 × 5 supercell of hBN with the lattice constant kept fixed at 5 × 2.504 Å while the atoms are fully relaxed without symmetry constraints. For calculations on monolayer hBN, a vacuum of 15 Å is used to avoid spurious interlayer interactions with the periodic replicas. We use ONCV pseudopotentials^{49,50} for all atoms, a planewave kinetic energy cutoff of 80 Ry and a 3 × 3 kpoint Brillouin zone grid. The GWBSE calculations are carried out with the Yambo code^{51,52} using a 2D slab cutoff of the Coulomb interaction. For calculations of defects in monolayer hBN, a 3 × 3 kpoint grid is employed together with an energy cutoff of 10 Ry for the dielectric matrix. The number of empty bands included in the GW calculation (for the polarizability and selfenergy summations) is 7 times the number of occupied bands. At least 6 valence and 6 conduction bands are included when diagonalizing the BSE matrix. These parameters converge the exciton energy to within 0.1 eV in our test calculations, which are shown in the Supplementary Note 1. For calculations on defects in bulk hBN, we use a 5 × 5 × 1 supercell containing two AA’stacked layers. The bulk case uses a 2 × 2 × 3 kpoint grid; all other parameters are the same as in the monolayer case.
Data availability
All data needed to evaluate the conclusions in the paper are present in the paper and/or the Supplementary Information. Additional data related to this paper may be requested from the authors.
References
Liu, X. & Hersam, M. C. 2D materials for quantum information science. Nat. Rev. Mater. 4, 669–684 (2019).
Chen, X. Entanglement of singlephotons and chiral phonons in atomically thin WSe_{2}. Nat. Phys. 15, 221–227 (2019).
Tran, T. T., Bray, K., Ford, M. J., Toth, M. & Aharonovich, I. Quantum emission from hexagonal boron nitride monolayers. Nat. Nanotechnol. 11, 37–41 (2016).
Gottscholl, A. Initialization and readout of intrinsic spin defects in a van der Waals crystal at room temperature. Nat. Mater. 19, 540–545 (2020).
Childress, L. Coherent dynamics of coupled electron and nuclear spin qubits in diamond. Science 314, 281–285 (2006).
Ladd, T. D. Quantum computers. Nature 464, 45–53 (2010).
Hensen, B. Loopholefree Bell inequality violation using electron spins separated by 1.3 kilometres. Nature 526, 682–686 (2015).
Aharonovich, I., Englund, D. & Toth, M. Solidstate singlephoton emitters. Nat. Photonics 10, 631–641 (2016).
Caldwell, J. D. Photonics with hexagonal boron nitride. Nat. Rev. Mater. 4, 552–567 (2019).
Jungwirth, N. R. Temperature dependence of wavelength selectable zerophonon emission from single defects in hexagonal boron nitride. Nano Lett. 16, 6052–6057 (2016).
Tran, T. T. Robust multicolor single photon emission from point defects in hexagonal boron nitride. ACS Nano 10, 7331–7338 (2016).
Dietrich, A. Observation of fourier transform limited lines in hexagonal boron nitride. Phys. Rev. B 98, 081414 (2018).
Tawfik, S. A. Firstprinciples investigation of quantum emission from hBN defects. Nanoscale 9, 13575–13582 (2017).
Weston, L., Wickramaratne, D., Mackoit, M., Alkauskas, A. & Van de Walle, C. G. Native point defects and impurities in hexagonal boron nitride. Phys. Rev. B 97, 214104 (2018).
Sajid, A., Reimers, J. R. & Ford, M. J. Defect states in hexagonal boron nitride: Assignments of observed properties and prediction of properties relevant to quantum computation. Phys. Rev. B 97, 064101 (2018).
LópezMorales, G. I., Proscia, N. V., López, G. E., Meriles, C. A. & V. M. Menon, Toward the identification of atomic defects in hexagonal boron nitride: Xray photoelectron spectroscopy and firstprinciples calculations. Preprint at https://arxiv.org/abs/1811.05924 (2018).
Noh, G. Stark tuning of singlephoton emitters in hexagonal boron nitride. Nano Lett. 18, 4710–4715 (2018).
Abdi, M., Chou, J. P., Gali, A. & Plenio, M. B. Color centers in hexagonal boron nitride monolayers: A group theory and ab initio analysis. ACS Photonics 5, 1967–1976 (2018).
Turiansky, M. E., Alkauskas, A., Bassett, L. C. & Van De Walle, C. G. Dangling bonds in hexagonal boron nitride as singlephoton emitters. Phys. Rev. Lett. 123, 127401 (2019).
Bernardi, M., Palummo, M. & Grossman, J. C. Extraordinary sunlight absorption and one nanometer thick photovoltaics using twodimensional monolayer materials. Nano Lett. 13, 3664 (2013).
Qiu, D. Y., Da Jornada, F. H. & Louie, S. G. Optical spectrum of MoS_{2}: Manybody effects and diversity of exciton states. Phys. Rev. Lett. 111, 216085 (2013).
RefaelyAbramson, S., Qiu, D. Y., Louie, S. G. & Neaton, J. B. Defectinduced modification of lowlying excitons and valley selectivity in monolayer transition metal dichalcogenides. Phys. Rev. Lett. 121, 167402 (2018).
Attaccalite, C., Bockstedte, M., Marini, A., Rubio, A. & Wirtz, L. Coupling of excitons and defect states in boronnitride nanostructures. Phys. Rev. B 83, 144115 (2011).
Reimers, J. R., Sajid, A., Kobayashi, R. & Ford, M. J. Understanding and calibrating densityfunctionaltheory calculations describing the energy and spectroscopy of defect sites in hexagonal boron nitride. J. Chem. Theory Comput. 14, 1602–1613 (2018).
V., Ivády, et al. Ab initio theory of the negatively charged boron vacancy qubit in hexagonal boron nitride. npj Comput. Mater. 6 (2020).
Rohlfing, M. & Louie, S. G. Electronhole excitations and optical spectra from first principles. Phys. Rev. B 62, 4927 (2000).
Palummo, M., Bernardi, M. & Grossman, J. C. Exciton radiative lifetimes in twodimensional transition metal dichalcogenides. Nano Lett. 15, 2794 (2015).
Chen, H.Y., Palummo, M., Sangalli, D. & Bernardi, M. Theory and ab initio computation of the anisotropic light emission in monolayer transition metal dichalcogenides. Nano Lett. 18, 3839 (2018).
Chen, H.Y., Jhalani, V. A., Palummo, M. & Bernardi, M. Ab initio calculations of exciton radiative lifetimes in bulk crystals, nanostructures, and molecules. Phys. Rev. B 100, 075135 (2019).
Jhalani, V. A., Chen, H.Y., Palummo, M. & Bernardi, M. Precise radiative lifetimes in bulk crystals from first principles: the case of wurtzite gallium nitride. J. Phys.: Condens. Matter 32, 084001 (2019).
R. Loudon, The Quantum Theory of Light (OUP Oxford, 2000).
Kimble, H. J., Dagenais, M. & Mandel, L. Photon antibunching in resonance fluorescence. Phys. Rev. Lett. 39, 691 (1977).
Hybertsen, M. S. & Louie, S. G. Electron correlation in semiconductors and insulators: Band gaps and quasiparticle energies. Phys. Rev. B 34, 5390 (1986).
Exarhos, A. L., Hopper, D. A., Grote, R. R., Alkauskas, A. & Bassett, L. C. Optical signatures of quantum emitters in suspended hexagonal boron nitride. ACS Nano 11, 3328–3336 (2017).
Hayee, F. Revealing multiple classes of stable quantum emitters in hexagonal boron nitride with correlated optical and electron microscopy. Nat. Mater. 19, 534–539 (2020).
Chejanovsky, N. Structural attributes and photodynamics of visible spectrum quantum emitters in hexagonal boron nitride. Nano Lett. 16, 7037–7045 (2016).
Choi, S. Engineering and localization of quantum emitters in large hexagonal boron nitride layers. ACS Appl. Mater. Interfaces 8, 29642–29648 (2016).
Cudazzo, P., Tokatly, I. V. & Rubio, A. Dielectric screening in twodimensional insulators: Implications for excitonic and impurity states in graphane. Phys. Rev. B 84, 085406 (2011).
Andersen, K., Latini, S. & Thygesen, K. S. Dielectric genome of van der Waals heterostructures. Nano Lett. 15, 4616–4621 (2015).
Von Toussaint, U. Bayesian inference in physics. Rev. Mod. Phys. 83, 943–999 (2011).
Mendelson, N. et al. Identifying carbon as the source of visible singlephoton emission from hexagonal boron nitride. Nat. Mater. (2020).
Bourrellier, R. Bright UV single photon emission at point defects in hBN. Nano Lett. 16, 4317–4321 (2016).
Tan, Q.H. et al. Ultraviolet to nearinfrared single photon emitters in hBN. Preprint at https://arxiv.org/abs/1908.06578 (2019).
Li, S. et al. Giant shift upon strain on the fluorescence spectrum of V_{N}N_{B} color centers in hBN. NPJ Quantum Information. 6, 85 (2020). https://www.nature.com/articles/s4153402000312y.
Jungwirth, N. R. & Fuchs, G. D. Optical absorption and emission mechanisms of single defects in hexagonal boron nitride. Phys. Rev. Lett. 119, 057401 (2017).
Mishra, H. & Bhattacharya, S. Giant excitonphonon coupling and zeropoint renormalization in hexagonal monolayer boron nitride. Phys. Rev. B 99, 165201 (2019).
Perdew, J. P., Burke, K. & Ernzerhof, M. Generalized gradient approximation made simple. Phys. Rev. Lett. 77, 3865 (1996).
Giannozzi, P. QUANTUM ESPRESSO: a modular and opensource software project for quantum simulations of materials. J. Phys. Condens. Matter 21, 395502 (2009).
Hamann, D. R. Optimized normconserving Vanderbilt pseudopotentials. Phys. Rev. B 88, 085117 (2013).
Schlipf, M. & Gygi, F. Optimization algorithm for the generation of ONCV pseudopotentials. Comput. Phys. Commun. 196, 36–44 (2015).
Marini, A., Hogan, C., Grüning, M. & Varsano, D. Yambo: an ab initio tool for excited state calculations. Comput. Phys. Commun. 180, 1392–1403 (2009).
Sangalli, D. Manybody perturbation theory calculations using the yambo code. J. Phys. Condens. Matter 31, 325902 (2019).
Acknowledgements
We acknowledge valuable discussions with Hamidreza Akbari. This work was supported by the Department of Energy under Grant No. DESC0019166. The radiative lifetime code development was partially supported by the National Science Foundation under Grant No. ACI1642443. H.Y.C. was partially supported by the J. Yang Fellowship. This research used resources of the National Energy Research Scientific Computing Center, a DOE Office of Science User Facility supported by the Office of Science of the US Department of Energy under Contract No. DEAC0205CH11231.
Author information
Authors and Affiliations
Contributions
S.G. and M.B. conceived and designed the research. S.G. performed calculation and analysis. H.Y.C. provided theoretical support. M.B. supervised the entire research project. All authors discussed the results and contributed to the manuscript.
Corresponding author
Ethics declarations
Competing interests
The authors declare no competing interests.
Additional information
Publisher’s note Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Supplementary information
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
Gao, S., Chen, HY. & Bernardi, M. Radiative properties of quantum emitters in boron nitride from excited state calculations and Bayesian analysis. npj Comput Mater 7, 85 (2021). https://doi.org/10.1038/s41524021005442
Received:
Accepted:
Published:
DOI: https://doi.org/10.1038/s41524021005442
This article is cited by

Exceptionally strong coupling of defect emission in hexagonal boron nitride to stacking sequences
npj 2D Materials and Applications (2024)

Electrical tuning of quantum light emitters in hBN for free space and telecom optical bands
Scientific Reports (2024)

Roomtemperature phononcoupled singlephoton emission in hexagonal boron nitride
Science China Physics, Mechanics & Astronomy (2024)

Strain tunable quantum emission from atomic defects in hexagonal boron nitride for telecombands
Scientific Reports (2022)

Computational design of quantum defects in twodimensional materials
Nature Computational Science (2021)